PHYSICAL REVIEW LETTERS

week ending 6 SEPTEMBER 2013

Generalized Model for Photoinduced Surface Structure in Amorphous Thin Films Chao Lu,1 Daniel Recht,2 and Craig Arnold1,* 1

Department of Mechanical and Aerospace Engineering, Princeton University, Princeton, New Jersey 08544, USA 2 School of Engineering and Applied Sciences, Harvard University, Cambridge, Massachusetts 02138, USA (Received 22 April 2013; revised manuscript received 2 August 2013; published 5 September 2013) We present a generalized model to explain the spatial and temporal evolution of photoinduced surface structure in photosensitive amorphous thin films. The model describes these films as an incompressible viscous fluid driven by a photoinduced pressure originating from dipole rearrangement. This derivation requires only the polarizability, viscosity and surface tension of the system. Using values of these physical parameters, we check the validity of the model by fitting to experimental data of As2 S3 and demonstrating good agreement. DOI: 10.1103/PhysRevLett.111.105503

PACS numbers: 81.65.b, 66.30.h, 68.35.Fx, 78.66.Jg

Introduction.—Photoinduced surface relief structures are generated in a variety of materials including azobenzene-containing polymers, chalcogenide glasses (like As2 S3 , AsSe, and GeAsSe), and other amorphous materials [1–5]. Macroscopic surface structures can be inscribed by illumination with a laser field having spatially varying intensity or polarization [6]. This phenomenon is potentially useful for technologies such as rewritable optical data storage, active optical devices, nanofabrication, and optical actuators [7]. However, to date a complete description of the underlying microscopic mechanism has not been produced. Much experimental and theoretical work has been performed to clarify the mechanism of this phenomenon. Models have been proposed to describe the formation of surface relief [3,8], where volumetric internal pressure, interaction among dipoles, anisotropic diffusion, or optical gradient forces were considered as the driving force for deformation [9–11]. These efforts have not led to a unified model that captures all experimental observations. Here we model surface relief formation as arising from viscous flow driven by the opposition of surface tension and an optically induced pressure which provides a driving force for mass transport that depends on both intensity and polarization. Accommodating both of these dependencies in a single model formulation is the main innovation of this work. Simulations using our model agree well with literature data on the temporal and spatial dependence of optically induced surface relief in As2 S3 . The model.—For simplicity and correspondence with past experiments we model a film of chalcogenide glass exposed to normal-incidence, time-independent, nearband-gap illumination that varies in one direction along its surface (the x axis) but is uniform along the other surface axis (y). At near-band-gap wavelengths films with thicknesses of order 1 micron or less are optically thin and so we take illumination to be uniform in the direction normal to the film’s surface (z) [12]. Figure 1 illustrates this coordinate system. We assume that the viscosity remains high enough to justify the low-Reynolds 0031-9007=13=111(10)=105503(5)

number lubrication approximation to the Navier-Stokes equations [13]. We further posit that surface tension and the optically induced pressure are the dominant forces. The above assumptions bring surface relief formation within the scope of the Navier-Stokes equation simplified into a two-dimensional boundary layer equation in x and z [14] (see Fig. 1). @vx @v @v 1 @P @2 v þ 2x þ f; þ vx x þ vz x ¼ @x @t @x @z @z

(1)

where the vi ’s are components of the velocity vector, is the mass density, P is the total pressure, f is the body force, and is the kinematic viscosity. Deriving the standard high-surface-tension lubrication equation in the presence of a pressure and absence of any body force yields @h @ h3 @PðxÞ @3 h s 3 ; (2) @t @x 3 @x @x in which hðx; tÞ is the film thickness, is the dynamic viscosity, s is the curvature coefficient of the surface tension, and PðxÞ is the optically induced pressure, which is assumed to vary only in x because that is the only

FIG. 1. Schematic of the typical experimental setup used to generate surface structure. Two beams, W1 and W2, interfere on the surface of a thin film of amorphous, light-sensitive material, leading to the pictured definitions of the coordinate system and polarization directions.

105503-1

Ó 2013 American Physical Society

week ending 6 SEPTEMBER 2013

PHYSICAL REVIEW LETTERS

PRL 111, 105503 (2013)

when exposed to the optical electric field. Rigorous results for the pressure are obtained from Eq. (3), in terms of the stress tensor ik ¼ 0 Ei Dk : FIG. 2 (color online). Schematic of photoinduced dipoles (on the scale of about 3 coordination spheres [19]) and their rearrangement leading to mass transport [22]. Dipoles can lower their energy by changing configurations in response to the optical electric field. In the case of linear polarization the dipoles will align with the optical electric field.

dimension in which the illumination is modulated [14–17]. The complete derivation can be found in the Appendix. Given a model of the optically induced pressure, Eq. (2) is readily solvable by standard numerical methods. Our model of the optically induced pressure is based on two assertions. First, the pressure arises from the electric field of the incident light. Second, the material responds through the motion of photoinduced dipoles. In the case of amorphous chalcogenides, each dipole corresponds to a group of atoms on the scale of 3 coordination spheres [18,19] which is capable of rearranging (i.e., mass transport) to change the orientation of the dipole (see Fig. 2). The experimental and theoretical literature indicate that these dipoles persist (fixed to the underlying atomic structure) as long as the illumination is present [19–22]. Moreover, although various mechanisms may generate photoinduced dipoles in different materials [20,23], the model applies as long as those dipoles R exist. The strength of the dipoles are given by P~ ¼ d3 rðr~Þr~, where the charge distribution ð~rÞ might be obtained from firstprinciples calculations [24]. To calculate the photoinduced pressure we start with the relation pressure / @ energy / @V. Equations describing the total free energy density of a dipole interaction system in the presence of an electric field are given by Landau [25], energy ¼ F0 þ ik 0 Ei Ek ;

(3)

where Ei and Ek are components of the electric field, F0 is the free energy of the system in the absence of an external field, ik is a component of the relative permittivity tensor, and Einstein notation has been used. In the dipole interaction model, ik describes the polarizability of the dipoles

Inserting Dk ¼ ðkm Em Þ into Eq. (4), yields ik ¼ 0 Ei ðkx Ex þ ky Ey þ kz Ez Þ:

IðxÞ=

s-s

2E2m ðxÞð1

p-p

2E2m ðxÞð1 þ cos2Þ

c ðxÞ ðxÞ

þ cos2Þ =2

s-p 45–135

2E2m ðxÞ 2E2m ðxÞ

LCP-RCP

2E2m ðxÞ

0

PðxÞ

0

ðc1 c2 Þ2E2m ðxÞð1 þ cos2Þ

0

ðc1 þ c2 Þ2E2m ðxÞð1 þ cos2Þ

=4 2 =2 0

(5)

Optical electric fields oscillate much faster than any time scale relevant to the flow and so the material must respond to the time average of the electric field. Thus, taking the trace of the stress tensor and calculating its time average, we can write the pressure as 1 1 P ¼ hTrðÞi ¼ hxx þ yy þ zz i 3 3 0 ¼ hEx ðxx Ex þ xy Ey Þ þ Ey ðyx Ex þ yy Ey Þi 3 0 (6) ¼ hxx E2x þ 2xy Ex Ey þ yy E2y i: 3 Noting that the material can respond only to the real part of the electric field, we require PðEx ; Ey Þ ¼ PðE~x ; E~y Þ where E~x ¼